#------------------------------------------------------------------------------
#$Date: 2015-01-27 21:58:39 +0200 (Tue, 27 Jan 2015) $
#$Revision: 130149 $
#$URL: svn://www.crystallography.net/cod/cif/1/00/01/1000105.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1000105
loop_
_publ_author_name
'Le Bail, A'
'Mercier, A M'
_publ_section_title              'Crystal structure of Pb₈MnFe₂F₂₄'
_journal_coden_ASTM              EJSCE5
_journal_name_full
;
European Journal of Solid State Inorganic Chemistry
;
_journal_page_first              183
_journal_page_last               190
_journal_volume                  29
_journal_year                    1992
_chemical_formula_structural     'Pb8 (Mn Fe2 F14) F10'
_chemical_formula_sum            'F24 Fe2 Mn Pb8'
_chemical_name_systematic
;
Octalead catena-fluorodiferrato(III)manganate(II) decafluoride
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 105
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   20.181(3)
_cell_length_b                   5.625(1)
_cell_length_c                   9.438(2)
_cell_volume                     1034.9
_refine_ls_R_factor_all          0.034
_cod_database_code               1000105
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
1/2-x,1/2+y,-z
-x,-y,-z
1/2+x,1/2-y,z
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_attached_hydrogens
_atom_site_calc_flag
Pb1 Pb2+ 4 e 0.08788(2) 0.00416(8) 0.44092(4) 1. 0 d
Pb2 Pb2+ 4 e 0.36846(2) 0.02402(9) 0.82663(4) 1. 0 d
Pb3 Pb2+ 4 e 0.17869(2) 0.00239(7) 0.90115(4) 1. 0 d
Pb4 Pb2+ 4 e 0.27492(2) 0.02257(9) 0.34946(4) 1. 0 d
Mn1 Mn2+ 2 a 0. 0. 0. 1. 0 d
Fe1 Fe3+ 4 e 0.45299(6) 0.0025(3) 0.2501(2) 1. 0 d
F1 F1- 4 e 0.2255(3) 0.2580(12) 0.1253(7) 1. 0 d
F2 F1- 4 e 0.2280(3) 0.7548(12) 0.1307(6) 1. 0 d
F3 F1- 4 e 0.1800(3) 0.2518(10) 0.3915(6) 1. 0 d
F4 F1- 4 e 0.1824(3) 0.7401(10) 0.3902(7) 1. 0 d
F5 F1- 4 e 0.1799(3) 0.9428(13) 0.6420(6) 1. 0 d
F6 F1- 4 e 0.3585(3) 0.0683(13) 0.1355(8) 1. 0 d
F7 F1- 4 e 0.4554(4) 0.2836(12) 0.3649(8) 1. 0 d
F8 F1- 4 e 0.0481(3) 0.5667(13) 0.3391(7) 1. 0 d
F9 F1- 4 e 0.0946(3) 0.9468(13) 0.1424(8) 1. 0 d
F10 F1- 4 e 0.4499(4) 0.7213(11) 0.1241(7) 1. 0 d
F11 F1- 4 e 0.0890(4) 0.3188(12) 0.6266(8) 1. 0 d
F12 F1- 4 e 0.4847(4) 0.1885(14) 0.1077(9) 1. 0 d
loop_
_atom_type_symbol
_atom_type_oxidation_number
Pb2+ 2.000
Mn2+ 2.000
Fe3+ 3.000
F1- -1.000
